Phase Formation, Microstructure and Mechanical Properties ... Phase Formation, Microstructure and...
Embed Size (px)
Transcript of Phase Formation, Microstructure and Mechanical Properties ... Phase Formation, Microstructure and...
590 Chiang Mai J. Sci. 2011; 38(4)
Chiang Mai J. Sci. 2011; 38(4) : 590-600 http://it.science.cmu.ac.th/ejournal/ Contributed Paper
Phase Formation, Microstructure and Mechanical Properties of ZrO2 Modified-Dental Porcelain Ceramics Attavit Pisitanusorn [a], Rattikorn Yimnirun [b], and Supon Ananta [c]* [a] Department of Prosthodontics, Faculty of Dentistry, Chiang Mai University, Chiang Mai 50200, Thailand. [b] School of Physics, Institute of Science, Suranaree University of Technology, Nakhon Ratchasima 30000,
Thailand. [c] Department of Physics and Materials Science, Faculty of Science, Chiang Mai University,
Chiang Mai 50200, Thailand. *Author for correspondence; e-mail: firstname.lastname@example.org
Recieved: 2 May 2011 Accepted: 21 June 2011
ABSTRACT The potential of a combination between single-step sintering and ZrO2 additive as a
simple ceramic fabrication method to obtain dental porcelain-based ceramic-nanocomposites with good mechanical properties was demonstrated. Influences of sintering condition on phase formation, densification, microstructure and mechanical properties of these porcelain ceramics were examined via XRD, SEM-EDX and Vickers indentation. It has been found that the choice of both sintering temperature and dwell time is one of the key factors controlling densification and leucite crystallization on the zirconia surface in dental porcelain ceramics.
Keywords: dental porcelain ceramics, leucite, sintering, strength.
1. INTRODUCTION Leucite glass-ceramics are one of the
significant restorative materials for dental applications owing to their suitable biocom- patibility, wear resistance and esthetics. However, similar to other glass-ceramics, a major disadvantage to dentistry of porcelain- based ceramics is their brittleness, which often deteriorates their utilization in fields where high strength and toughness are required [1,2]. Several approaches have been introduced to minimize this limitation and improve the mechanical properties including a method of reinforcing the glassy matrix with high strength
crystalline phases such as alumina (Al2O3), zirconia (ZrO2) or leucite (KAlSi2O6) [2-4]. A significant milestone in this respect was established in the development of dental ceramics containing leucite crystalline phase because of their excellent thermal compatibility when bonding to metals and also a reinforcing agent in all ceramic restorations [5-7]. In general, most commercial porcelains for dental restorations are partially crystallized feldspathic glasses that consist of tetragonal-leucite crystals embedded in a glassy matrix. It has been reported that leucite glass-ceramics can
Chiang Mai J. Sci. 2011; 38(4) 591
be fabricated by controlled crystallization of a glass via leucite additive, heat treatment and etc. [8-9]. In general, commercial dental porcelain ceramics contain some amount of leucite crystals sized ~5-10 μm causing extensive microcracking around these non- uniformed leucite crystals . To overcome these problems, several efforts have been made to tailor the leucite morphology, volume fraction and distribution which is thought to affect the mechanical properties of these porcelain ceramics via heat treatment [4,9] or heat pressing .
According to a study on the effects of multiple firing and isothermal anneals on the leucite volume fraction reported by Mackert and Evan , it is established that measurable changes in the leucite concentration exist upon a variety of porcelain heat treatments. Although the study on the formation of leucite crystalline in porcelains has been reported by several researchers [7-9]; so far, attentions directly paid on the Zr-modified porcelain- based ceramics are very few. In connection with this, our earlier works  have demonstrated that the two-step sintering technique together with 20-wt% ZrO2 additive has considerable potential for the production of leucite/porcelain ceramic-nanocomposites. It was also found that the tempering time is a key factor to controlling dendritic morphology of leucite crystallization behavior and microstructural arrangement in ZrO2- modified dental porcelain ceramics. However, no information regarding the mechanical properties of these materials is available. Moreover, effects of single-step sintering for the production of ZrO2-modified dental porcelains have not yet been adequately characterized. Thus, in the present study, dental porcelain ceramics were fabricated by using both a single-step sintering and 20 wt% ZrO2 additive techniques. Their mechanical properties with respect to both firing
temperature and dwell time were investigated, compared and explained on the basis of their composition, densification, and microstructural evolution.
2. MATERIALS AND METHODS The starting materials were commercially
available dental porcelain powders (Vita- VMK95, Vita Zahnfabrik, Bad S ckingen, Germany), which had particle size range of ~1.5-2.5 μm. Porcelain powders were mixed with 20 wt% of zirconia powders (Sigma- Aldrich, purity > 99%) by using a rapid vibro-milling for 30 min [2,12]. The methods of mixing, drying, grinding and sieving of the products were similar to those employed in the preparation of the alumina-modified dental porcelain powders as described previously [2, 12]. Green samples were obtained by mixing powders with polyvinyl alcohol binder (PVA) via a slip-casting technique as recommended by the manufacturer , and then poured into a standard stainless steel mould with a normal-sized cavity of 30 mm × 6 mm × 2 mm, reproducing the desired dimensions and shapes [2, 12]. After moulding, the ceramics were fabricated by employing different firing schemes with heating rate of 25oC/min in a vacuum furnace (Multimat Touch & Press, Germany), with details listed in Table 1. During heating, the temperature was maintained at 500oC for 1 h to burn out the PVA binder. The dental porcelain, i.e. the control group (D0), was sintered at 1,060oC for 5 min. Further increase in the soaking time longer than 5 min results in melted samples probably due to a liquid-phase formation during the sintering process of dental porcelains . The other groups of samples (coded D1-D9) were sintered by employing various firing temperature and dwell time. In contrast to those adopted by Chayada et al. , in this work, no second firing-step and quenching processes are required. Densities of
592 Chiang Mai J. Sci. 2011; 38(4)
the final sintered products were determined by using the Archimedes principle. Phase formation and microstructural were examined by room temperature X-ray diffraction analysis (XRD; X’pert MPD, Philips Corp, Japan) using Ni-filtered Cu Kα radiation and field emission scanning electron microscopy (SEM; JSM-840A 6335 F, Jeol, Japan), respectively. The mean crystallite size was determined using the diffraction peak (400) of the leucite pattern by using Scherrer equation . Lattice parameters of the leucite phase were determined from the d spacing for the (400) and (004) peaks for the tetragonal phase [4,12]. The grain size and morphologies of leucite phase in the sintered samples were determined from SEM micrographs. The chemical composition of the phase formed was also elucidated by an energy dispersive X-ray (EDX) analyzer with an ultra-thin window. EDX spectra were quantified with the virtual standard peaks supplied with the Oxford Instruments eXL software. In order to evaluate the mechanical properties of these samples, the characterization methods previously described in our earlier works  were performed. The uniaxial flexural strength was measured with the three-point bending technique and calculated as recommended by ISO 6872. Hardness and Young’s modulus were determined and calculated for all materials by the Vickers microhardness testing machine, and were measured as recommended by the ASTM C 1327-99 and C 1259-01, respectively. Fracture toughness was assessed using the indentation strength method. Hardness and elastic modulus are parameters of the equation used for calculation of the fracture toughness. The fracture toughness was calculated with the equation proposed by Fischer and Mark .
3. RESULTS AND DISCUSSION The densification, leucite crystallization,
microstructural evolution and mechanical behavior of the Zr-modified dental porcelain ceramics subjected to various sintering conditions are given in Table 1. In the sintering temperature range of 1,060-1,140oC, the density increases with increasing temperature. For a given sintering temperature, similar trend of the density is also observed with the extending of dwell time from 20 to 30 min. However, it can be seen that further increase in the dwell time to 40 min leads to the decrease of the density. This feature creates a maximum density value of about 2.88 g/cm3 which is comparable to the values reported by Chayada et al. (~2.76 g/cm3 ) where the two-step sintering technique was used. The increasing density with rising dwell time up to 30 min may be explained by the enhanced densification related to the effect of ZrO2 [3, 12]. Further increase in the dwell time causes a decrease in density values. This may be attributed to the suppression of atomic diffusion at probably too long soaking times resulting in an incomplete densification [12, 17]. Similar behavior is also reported by Chayada et al.  for zirconia-modified dental porcelains derived from the two-step sintering technique. As is well known, the difference in thermal expansion between the tetragonal leucite crystals and the glassy matrix also provides tangential compressive stresses around the crystals that are thought responsible for significant strengthening in dental porcelain [4, 9]. The crystallization of a high expansion te